LMucko/crystallography-open-database huggingface dataset:
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 1st run, T = 200 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007116
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 1st run, T = 200 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0950
_cell_length_b                   8.0950
_cell_length_c                   8.0950
_cell_formula_units_Z            8
_cell_volume                     530.457
_database_code_amcsd             0008701
_diffrn_ambient_temperature      473.15
_exptl_crystal_density_diffrn    3.563
_exptl_crystal_thermal_history   'heating, 1st run, T = 200 C'
_cod_original_cell_volume        530.458
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007116
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 1st run, T = 400 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007117
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 1st run, T = 400 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1092
_cell_length_b                   8.1092
_cell_length_c                   8.1092
_cell_formula_units_Z            8
_cell_volume                     533.254
_database_code_amcsd             0008702
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    3.544
_exptl_crystal_thermal_history   'heating, 1st run, T = 400 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007117
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 1st run, T = 25 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007118
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 1st run, T = 25 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0849
_cell_length_b                   8.0849
_cell_length_c                   8.0849
_cell_formula_units_Z            8
_cell_volume                     528.474
_database_code_amcsd             0008703
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    3.576
_exptl_crystal_thermal_history   'heating, 1st run, T = 25 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007118
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 2nd run, T = 500 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007119
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 2nd run, T = 500 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1169
_cell_length_b                   8.1169
_cell_length_c                   8.1169
_cell_formula_units_Z            8
_cell_volume                     534.774
_database_code_amcsd             0008704
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.534
_exptl_crystal_thermal_history   'heating, 2nd run, T = 500 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007119
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 2nd run, T = 400 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007120
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 2nd run, T = 400 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1095
_cell_length_b                   8.1095
_cell_length_c                   8.1095
_cell_formula_units_Z            8
_cell_volume                     533.313
_database_code_amcsd             0008705
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    3.544
_exptl_crystal_thermal_history   'heating, 2nd run, T = 400 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007120
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 3rd run, T = 550 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007121
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 3rd run, T = 550 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1204
_cell_length_b                   8.1204
_cell_length_c                   8.1204
_cell_formula_units_Z            8
_cell_volume                     535.466
_database_code_amcsd             0008706
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    3.529
_exptl_crystal_thermal_history   'heating, 3rd run, T = 550 C'
_cod_original_cell_volume        535.467
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007121
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 3rd run, T = 600 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007122
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 3rd run, T = 600 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1251
_cell_length_b                   8.1251
_cell_length_c                   8.1251
_cell_formula_units_Z            8
_cell_volume                     536.397
_database_code_amcsd             0008707
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    3.523
_exptl_crystal_thermal_history   'heating, 3rd run, T = 600 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007122
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 3rd run, T = 700 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007123
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 3rd run, T = 700 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1336
_cell_length_b                   8.1336
_cell_length_c                   8.1336
_cell_formula_units_Z            8
_cell_volume                     538.082
_database_code_amcsd             0008708
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    3.512
_exptl_crystal_thermal_history   'heating, 3rd run, T = 700 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007123
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 3rd run, T = 800 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007124
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 3rd run, T = 800 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1407
_cell_length_b                   8.1407
_cell_length_c                   8.1407
_cell_formula_units_Z            8
_cell_volume                     539.492
_database_code_amcsd             0008709
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    3.503
_exptl_crystal_thermal_history   'heating, 3rd run, T = 800 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007124
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 3rd run, T = 900 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007125
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 3rd run, T = 900 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1485
_cell_length_b                   8.1485
_cell_length_c                   8.1485
_cell_formula_units_Z            8
_cell_volume                     541.045
_database_code_amcsd             0008710
_diffrn_ambient_temperature      1173.15
_exptl_crystal_density_diffrn    3.493
_exptl_crystal_thermal_history   'heating, 3rd run, T = 900 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007125
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Heating, 3rd run, T = 950 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007126
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Heating, 3rd run, T = 950 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1516
_cell_length_b                   8.1516
_cell_length_c                   8.1516
_cell_formula_units_Z            8
_cell_volume                     541.662
_database_code_amcsd             0008711
_diffrn_ambient_temperature      1223.15
_exptl_crystal_density_diffrn    3.489
_exptl_crystal_thermal_history   'heating, 3rd run, T = 950 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007126
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Cooling, T = 900 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007127
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Cooling, T = 900 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1474
_cell_length_b                   8.1474
_cell_length_c                   8.1474
_cell_formula_units_Z            8
_cell_volume                     540.825
_database_code_amcsd             0008712
_diffrn_ambient_temperature      1173.15
_exptl_crystal_density_diffrn    3.494
_exptl_crystal_thermal_history   'heating Sample: SYN, Cooling, T = 900 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007127
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Cooling, T = 800 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007128
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Cooling, T = 800 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1395
_cell_length_b                   8.1395
_cell_length_c                   8.1395
_cell_formula_units_Z            8
_cell_volume                     539.254
_database_code_amcsd             0008713
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    3.505
_exptl_crystal_thermal_history   'heating Sample: SYN, Cooling, T = 800 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007128
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Cooling, T = 800 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007129
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Cooling, T = 800 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1391
_cell_length_b                   8.1391
_cell_length_c                   8.1391
_cell_formula_units_Z            8
_cell_volume                     539.174
_database_code_amcsd             0008714
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    3.505
_exptl_crystal_thermal_history   'heating Sample: SYN, Cooling, T = 800 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007129
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Cooling, T = 700 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007130
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Cooling, T = 700 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1316
_cell_length_b                   8.1316
_cell_length_c                   8.1316
_cell_formula_units_Z            8
_cell_volume                     537.685
_database_code_amcsd             0008715
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    3.515
_exptl_crystal_thermal_history   'heating Sample: SYN, Cooling, T = 700 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007130
X-ray single-crystal study of spinels: in situ heating Sample: SYN, Cooling, T = 600 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007131
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: SYN, Cooling, T = 600 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1233
_cell_length_b                   8.1233
_cell_length_c                   8.1233
_cell_formula_units_Z            8
_cell_volume                     536.040
_database_code_amcsd             0008716
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    3.526
_exptl_crystal_thermal_history   'heating Sample: SYN, Cooling, T = 600 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Al2 Mg) O4'
_cod_database_code               9007131